EUTECTIC TRANSFORMATION IN DUCTILE CAST IRON. PART I THEORETICAL BACKGROUND


 Kellie Washington
 1 years ago
 Views:
Transcription
1 METALLURGY AND FOUNDRY ENGINEERING Vol. 31, 005, No. Edward Fraœ *, Marcin Górny **, Hugo F. López *** EUTECTIC TRANSFORMATION IN DUCTILE CAST IRON. PART I THEORETICAL BACKGROUND SYMBOLS Symbols Meaning Definition Units a Material mould ability to absorb of heat a = kmcm J/(cm ºC s 1/ ) A Parameter Eq. (10) s 1/ /m b Nucleation coefficient of graphite Eq. (58) o C B Temperature parameter Eq. (14) c Specific heat of metal Table 1 J/(cm 3 ºC) c m Specific heat of mould material J/(cm 3 ºC) C Carbon content in cast iron wt. % C e Carbon content in graphite eutectic Eq. () wt. % CT Chilling tendency Eqs. (67), (68) s 1/ / o C 1/3 C, C 3, C 4, C gr Carbon content in austenite, liquid and graphite Fig (3b) wt. % D Diffusivity of carbon in austenite Eq. (64) cm /s f gr Fraction of preeutectic graphite Eq. (1) * Prof., ** Ph.D., Faculty of Foundry Engineering, AGH University of Science and Technology, Cracow, Poland; ** Author is an award holder of the NATO Science Fellowship Programme *** Prof., Department of Materials Engineering, University of WisconsinMilwaukee, P.O. Box 784, Milwaukee, WI 5301, USA; 113
2 F c Surface area of the casting cm F ch Half surface area chill triangle Figure11 cm k Coefficient Eqs. (39), (43) k m Heat conductivity of the mould material J/(s cm ºC) l s l Size of substrate for nucleation of graphite Mean size of substrates for nucleation of graphite cm cm L e Latent heat of graphite eutectic Table 1 J/cm 3 m gr Mass of graphite Eq. (31) g m l Mass of graphite in liquid Eq. (30) g m γ Mass of graphite in austenite Eq. (35) g M Casting modulus Eqs. (11), (5), (55) cm M cr Critical casting modulus Eq. (70) cm N Volumetric nodule count Eqs. (57), (6) cm 3 N s Density of substrates for nucleation of graphite cm 3 P cr Coefficient Eq. (66) (cm o C 1/3 )/s 1/ P Phosphorus content in cast iron wt. % q a Accumulated heat flux in casting Eq. (6) J/s q m Heat flux extracted from casting into mould casting Eq. (5), (50) J/s q s Heat flux generated during solidification Eq. (7),(49) J/s Q Metal cooling rate Eq. (15) ºC/s R 1 Graphite nodule radius Figure 3b cm R Outer radius of austenite envelope Figure 3b cm R m Austenite envelope radius at maximum undercooling Eq. (47) cm s Wall thickness cm s cr Critical wall thickness Eqs. (71), (7) cm Si Silicon content in cast iron wt. % 114
3 t Time s t m Time at the maximum undercooling Eq. (1) s t s Time at the onset of graphite eutectic solidification s T Temperature ºC T c Equilibrium temperature of the cementite eutectic Table 1 ºC T i Initial temperature of metal in mould cavity ºC T m Temperature at maximum undercooling of graphite eutectic Figure a ºC T p Pouring temperature ºC T s Equilibrium temperature of the graphite eutectic Table 1 ºC V c Volume of casting cm 3 z Parameter Eq. (54) α Wedge angle Figure 11 o α d Thermal diffusivity of mould material k m /c m cm /s β Coefficient Table 1 o C 1 ΔH Enthalpy of metal J/cm 3 ΔΤ Undercooling of graphite eutectic ΔΤ m Maximum undercooling of graphite eutectic ΔΤ m = T s T m ºC ΔΤ sc Range of temperature, ΔΤ sc = T s T c Table 1 ºC θ Wetting angle between substrate and nuclei of graphite o ρ l Density of melt Table 1 g/cm 3 ρ gr Density of graphite Table 1 g/cm 3 ρ γ Density of austenite Table 1 g/cm 3 σ Interfacial energy between the nucleus and the melt J/cm ϕ, ϕ 1 Parameters Eqs. (5), (6) % ω Frequency Eq. (17) 1/s 115
4 1. INTRODUCTION Ductile cast iron is a modern engineering material whose production is continually increasing. Hence, there are numerous reports related to the production of nodular cast iron, some of which are of essential importance as they are linked to the solidification kinetics. In ductile cast iron, solidification is closely related to the nucleation and growth of nodular graphite. Yet, nucleation is the dominant process at the onset of solidification and it establishes the final nodule count. Accordingly, increasing the nodule count in a given cast iron leads to: Increasing strength and ductility in ductile cast iron [1]. Reduction of microsegregation of alloying elements [, 3], and improving microstructural homogeneity. Here, the type of eutectic transformation (stable or metastable) is also influenced due to the redistribution of alloying elements. Reduction in the chilling tendency of cast iron [4, 5]. Increasing preshrinkage expansion [6]. Increasing formation of open and closed contraction cavity volumes [7]. Increasing fraction of ferrite in the microstructure [8]. The chilling tendency (CT) of cast iron dictates their subsequent performance in diverse applications. In particular, cast iron possessing a high chilling tendency is prone to develop zones of white or mottled iron. Considering that, these regions can be extremely hard, their machinability can be severely impaired. Alternatively, if white iron is the desired structure a relatively small chilling tendency favours the formation of grey iron. This in turn leads to poor hardness and wear properties for the cast components. Hence, considerable efforts have been made in correlating various factors of technological relevance (inoculation practice, iron composition, pouring temperature, etc.) with the chill of cast iron. In this work, a simple analytical model of eutectic transformation in ductile cast iron is proposed. The model enables the determination of nodule counts in nodular cast iron, the chilling tendency CT and chill of ductile cast iron.. ANALYSIS Ductile cast iron is often hypereutectic, where the volume fraction of preeutectic graphite f gr is given by fgr ( C C ) ρl e = 100 ρgr Ceρ l + C( ρl ρgr) (1) where Ce = Si 0.36P () The influence of carbon and silicon on the preeutectic volume fraction of graphite is shown in Figure 1. From this figure it can be observed that for a useful C and Si range in the 116
5 foundry practice f gr ranges from 0 to 0.0; as a result, solidification of preeutectic graphite can be neglected. In this case, during solidification, heat extraction leads to changes in the relative energies of solid and liquid in two ways: 1) a reduction in the enthalpy of the liquid or solid due to cooling given by Ä H = cdt, ) a release heat of the eutectic solidification through the enthalpy contribution, known also as the latent heat (L). Hence, the heat transfer process can be described by the heat balance equation Fig. 1. Effect of carbon and silicon on the volumetric fraction of preeutectic graphite in hypereutectic cast iron qm = qs + qa (3) Heat transfer during solidification can be very complex and analytical solutions are not always available, so numerical methods are commonly employed. However, in sand castings, heat transfer is mainly determined by the properties of the sand mold as shown by Chvorinov [9]. a) b) T i a) mould b) Temperature T s T m I II ΔT m Temperature metal T i t s t m Time Fig.. Cooling curve for eutectic ductile cast iron (a) and temperature profile in the moldmetal system (b) Figure b shows the ideal temperature profile expected for sandmould metal systems. The heat flux going into the mold can be described by qm = Tkm ð á d t (4) 117
6 Taking into account the thermal diffusivity α d = k m /c m and the surface area F c of the casting, Eq. (4) can be rearranged as aft c qm = ð t (5) where a = k c. m m The above expression neglects curvature effects associated with the metalmold interface. Moreover, it is assumed that the temperature distribution along the metal is uniform. Hence, the accumulated heat flux in the metal can be described by cvc dt qa = dt (6) The heat flux q s generated during solidification depends on the particular solidification mechanism and in the present work it can be described by dv qs = LeNVc dt (7) where dv/dt is the volumetric solidification rate of eutectic cells (cm 3 /s). During solidification, two main stages can be distinguished (Fig. a). First Stage In this stage, the temperature of the melt decreases from T i to the equilibrium temperature for graphite eutetctic T s with no solidification events (Fig. a). Accordingly, q s = 0 and Eq. (3) can be rewritten as q m = q a (8) Taken into consideration Eqs. (5) and (6) and solving Eq. (8) for the initial conditions: T = T i at t = 0, the temperature during this stage is given by t T = Ti exp AM where: A = c π a (9) (10) M V = F c c (11) 118
7 Differentiating Eq. (9) yields an equation for the cooling rate as dt dt T i t = exp AM t A M (1) For t = t s, T = T s, and the time elapsed during the first stage can be found from Eq. (9) t s = (A B M) (13) where B = T ln i Ts (14) The metal cooling rate at the end of first stage can be calculated by taking into account Eqs. (1) (14) for t = t s, T = T s condition and after rearranging, yielding 1) dt Ts a = Q = dt (15) π Bc M Second Stage During this stage, the solidification of graphite eutectic occurs in the t s < t < t m time range or in the T s < T < T m temperature range (Fig. a). The initial segment of the cooling curve where the eutectic transformation takes place can be defined as a function of the degree of maximum undercooling ΔT m = T s T m (Fig. a). The solidification temperature for this temperature range can be described by [10] ( ) T = Ts ΔTmsin ω t ts (16) where ω= π ( t t ) m s (17) Equation (16) is of empirical nature. However it has been shown to provide an excellent description of the experimental outcome [10]. Accordingly, during second stage the cooling rate can be found by differentiating Eq. (16). dt dt = ΔTmωcos[ ω( t ts)] (18) 1) It is assumed that cooling rate has positive sign. 119
8 Therefore at the beginning of stage II when t = t s, cos0 = 1, the cooling rate can be described by ) dt Q = =ω Δ Tm (19) dt Combining Eqs. (17) and (19), and rearranging, yields ΔTm ( t t ) m s = Q π (0) At the onset of eutectic solidification (t = t s ), the cooling rates in the first and second stages it can be assumed equal each other. Therefore, using Eqs. (13), (15), and (0), the time for the maximum undercooling can be determined from t m ( +π Δ ) π Bc M BTs T = 4 a T s m (1) Nuclei N of nodular graphite are formed in the casting volume of liquid V c, and from each nucleus rise a single eutectic cell of spherical shape. Hence, the volume of the eutectic 3 cell with radius R (Fig. 3b) is given by V = (4 π R ) /3, while the differential volume increment is given by dv = 4 π R dr. Accordingly, taking into account Eq. (7) the expression for the rate of heat generation can be described by 4 π Le N Vc R dr q s = dt () In order to determine the radius R, as well as the growth rate of the cell, dr /dt the eutectic transformation in nodular cast iron will now be considered. Taking into account diffusional transport during the eutectic transformation and assuming spherical geometry (Fig. 3), the steady state solution for carbon diffusion through the austenite shell can be defined by solving equation dc d C D + = 0 rdr dr (3) ) It is assumed that cooling rate has positive sign. 10
9 a) b) Temperatue T s J ' E B C D graphite austenite R 1 R T ΔT m S C C 3 C 4 Carbon content C gr C 4 C C 3 Fig. 3. Schematic representation of a FeC phase diagram section (a) and corresponding carbon profile for a spherical eutectic cell (b) The general solution to the above equation yields ϕ C =ϕ+ r 1 (4) where r is the radial coordinate, R 1 < r < R and ϕ and ϕ 1 are constants which can be determined from the boundary conditions: C = C 3 at r = R and C = C at r = R 1. This yields: R1(C C 3) ϕ= C3 R R 1 RR 1 (C C 3) ϕ 1 = R R 1 (5) (6) Hence, taking into account Eqs. (4), (6) the solute concentration profile in the austenite envelope can be described by: ( C C )( ) R1 3 r R C( r) = C3 r ( R R1) (7) Moreover, deriving Eq. (7) with respect to r yields the carbon concentration gradient in the austenite envelope at the liquid austenite interface. dc R1 R (C C 3) = dr r ( R1 R) (8) 11
10 Also, at the austenite solidification interface r = R, the concentration gradient becomes dc R1(C3 C ) = dr R R R ( ) 1 (9) Introducing a mass balance in the diffusional system (Fig. 3b) where (C 4 ) is the carbon content in the volume (4πR 3 )/3 prior to the eutectic transformation (when only liquid is the stable phase). In this case, the mass of carbon in the liquid can be given by ml 4 3 = π R C4 (30) 3 After the eutectic transformation, the diffusional system is depicted by a graphite nodule of radius R 1 and concentration C gr surrounded by an austenite envelope of radii R 1 and R. The mass of carbon in the graphite nodule can be determined from mgr 4 3 = π R1 Cgr (31) 3 A differential increment in the volume of the austenite envelope dv = 4πr dr causes a differential increment in the carbon mass according to dm γ = 4 π C( r) r dr (3) Also, the carbon mass in the austenite envelope is described by R R1 mγ = 4 π C() r r dr (33) Considering Eqs. (7) and (33) and rearranging terms yields mγ = π C3R C R1 R1 R(C3 C )( R R1) 3 + (34) In the above equation, the third term within brackets is relatively small and can be neglected. This yields 3 3 ( C3 C 1 ) 4 mγ = R R 3 π (35) 1
11 From the mass balance (m l = m gr + m γ ), based on Eq. (30), (31) and (35) R 1 is found as 1/3 C4 C R 3 1 R = Cgr C (36) In addition, the condition for continuity across the liquid austenite interface needs to be taken into account. This condition using Fick law can be written as (C 4 dr dc C 3) D dt = dr (37) Combining Eqs. (9), (36), and (37) yields RdR = kddt (38) where k = ( ) (C C ) 3 C C gr C4 C3 3 1 C4 C3 (39) The above expression can be correlated with the degree of undercooling, ΔT. Assuming that the JE, E S and BC lines for the FeC system (Fig. 3a) are straight the concentrations in Eq. (39) can be given by: ΔT C = C E ' (40) m ΔT C3 = C E ' + (41) m 3 ΔT C4 = C C ' + (4) m 4 where: m, m 3 and m 4 are the slopes of the solubility lines JE, E S and BC respectively. 13
12 For FeC alloys the following values can be employed: C C = 4.6%, C E =.08%, m = 75 o C / %, m 3 = o C / %, and m 4 = = 113. o C / %. Using this data, estimations of k values are plotted in Figure 4. From this figure, it is apparent that k tends to exhibit a linear trend with ΔT. Accordingly, k can be described by k = β ΔT (43) where β = o C 1. Moreover, it can be shown that the effect of Si on β is negligible. In addition, considering that the degree of undercooling ΔT = T s T, from Eqs. (16), (38) and (43), it is found that Fig. 4. Graphic plot of Eq. (39) function as a function of the degree of undercooling, ΔT ( ) R dr =βd ΔTmsin ω t ts dt (44) Hence, integrating the above expression for the limiting conditions t = t s at R = 0, yields β D ΔT R m = 1 cos ω t ts ω ( ) 1/ (45) Differentiating Eq. (45) with respect to time yields the rate of eutectic cell growth 1/ dr β D ωδt m = sin ω( t ts ) dt 1 cos ( t t ω s ) (46) Then, at the time t = t m, and by taking into account Eq. (17), expressions for the cell radius, as well as the cell growth rate at the maximum undercooling are found: 1/ β D ΔT R m, m = ω (47) 1/ dr, m β D ω ΔTm = dt (48) 14
13 In addition, by taking into account Eqs. (10), (13), (17), (1), (), (47) and (48), the heat flux generated during solidification at the time t = t m is given by cm qs = 4 LeN Vc a ( ) B ΔTm π β D ΔTm T s 3 1/ (49) Moreover, combining Eqs. (3) and (1) for the same time t = t m, the heat flux going into the mold can be described by 3/ Fc a T q s m = 1/ 1/ π cm B ( π Δ Tm + Ts B) (50) At t = t m, the cooling rate is zero and as a consequence the rate of heat accumulation q a is also zero. Hence, the heat balance equation (Eq. (3)) becomes qs = qm (51) Finally, by taking into account Eqs. (11), (1), (49) and (51) an expression for the modulus of casting can be obtained. M 1/3 a T s = 1/ 5/ 1/ ( Dβ) π BNLe c ΔTm ( π Δ Tm + TB s ) (5) In nodular cast iron, the pouring temperature, T p ranges from 150 to 1450 o C. Hence, taking into account that T p = T i, typical B values (Eq. (14)) range from to 0.3. Figure 5 shows graphically the ( ) 1/ 1/ ΔTm π Δ Tm + TsB and z Δ TmTs functions versus ΔT m for two extreme values of B. From this figure it is evident that ( ) 1/ m m s s 1/ m ΔT π Δ T + T B z T Δ T (53) where z = B (54) Accordingly, taking into account Eqs. (5) and (53), N can be simplified to the following form M 1/ Ts 1 = a D 5/ β π zbnleδt m 1/3 (55) 15
14 a) b) m m s Δ π Δ + (solid line) and line) functions for: a) B = 0.074; b) B = 0.3 Fig. 5. Influence of ΔT m and B on the T ( T B T ) 1/ 1/ z Ts Δ Tm (dotted 3. NODULE COUNT Eq. (55) can be rewritten as a function of the cooling rate (taking into account Eq. (15)) as 1/ cb Q N = 1/ 4 π z L D e ΔT β m 3/ (56) The nucleation of graphite during solidification is of heterogeneous nature, on preferential substrates of various sizes, l s. The active substrate set is randomly distributed in the undercooled melt and it can be given by the substrate volume density, N s. A simple heterogeneous nucleation model previously developed [11] is employed in this work. Accordingly, the volume density of graphite nodules can be given by b N = Ns exp ΔT m (57) where 4 Ts σ sin θ b = Le l (58) Combining Eqs. (56) and (57) yields 1/ b c B Q Ns exp = ΔT π Δ D β 1/ m 4 z Le Tm 3/ (59) From this equation, the maximum degree of undercooling can be determined from Δ Tm = b ProductLog ( y) (60) 16
15 where 1/ 3 3 1/4 π zns Le D β y = b c 3 BQ (61) The ProductLog[y] = x is the Lambert function 3), also is called the omega function and it is graphically shown in Figure 6. This function is used to solve equation of the x type of y = xe. Its exact values can be easily calculated using the instruction of the ProductLog[y] in the Mathematica programme. In our analysis typical values of variable y are situated within boundaries from 0.03 to 500, and in case if we cannot Fig. 6. Graphic representation of the ProductLog[y] function for y 0 use Mathematica programme its value can be calculated by means of elementary mathematics with an accuracy higher than 99% using the following equations: for 0.03 y 1 range y x = ; y y for 1 y 5 range x= log( ) y y ; for 5 y 0 range x= log( ) y y ; for 0 y 50 range x= log( ) y y ; for 0 y x= log( ) y y. From Eqs. (57) and (60) N can be given by N N = s exp ProductLog( y) In metallographic determinations, the area density of graphite nodules N F is commonly measured at a given microsection. In addition, in ductile iron the graphite nodules are cha (6) 3) See 17
16 racterized by Raleigh distributions [1]. In this case the volumetric nodule count (N) can be related to the area nodule count (N F ) using the Wiencek equation [13] ( ) 1/3 gr NF = f N (63) where f gr is the volume fraction of graphite in eutectic, f gr = According to the literature, the nodule count N F is influenced by the chemical composition and the superheat temperature and time [14]. Yet, in the industrial practice, a drastic increase in nodule counts is usually obtained by the introduction of inoculants. In this case, the nodule count depends on the type of inoculant, quantity and granulation, Mg treatment and inoculation temperature, and the time after inoculation [14]. Also, it is well known that an increase in the cooling rates causes a radical increase in the nodule count in castings. From Eqs. (60) and (61) it can be seen that among the various factors that influence the final nodule count are: The diffusion coefficient of carbon in austenite, D depends on the actual temperature and chemical composition of the austenite. The effect of Si, Mn and P on D is not considered in this work as there is not enough information available in the literature. An expression for the diffusion coefficient of carbon in austenite has been published [15] D = exp , cm /s T T (64) During the eutectic transformation, the temperature, T ranges from to K, so the effective D values ranges from to cm /s. Therefore, an average D value of cm /s can be used without introducing significant error. In general, as D increases, the nodule count decreases as predicted by Eqs. (61) (11), (also see Fig. 7). Nucleation susceptibilities. Depending on the graphite nucleation susceptibilities in ductile cast iron at a given cooling rate, various nodule counts can be achieved. The nucleation susceptibilities of cast iron (Tab. 1) are characterized by N s and b. These coefficients (see Tab. 4, Part II) depend on the chemical composition, spheroidization practice, inoculation, and holding time of bath and temperature. Fig. 7. Influence of the diffusion coefficient for carbon in austenite on the nodule count; L e = 08.8 J/cm 3 ; c = 5.95 J/(cm 3 oc); β = o C 1 ; C = 3.71%, Si =.77%, P = 0.034%; T i = 1300 o C; D = = cm /s (rest of data see Tab. 1) 18
17 Table 1. Physicalchemical data for nodular cast iron Latent heat of graphite eutectic L e = 08.8 J cm 3 Specific heat of the cast iron Coefficient of heat accumulation by the mould material c = 5.95 J cm 3 o C a = 0.1 J cm s 1/ o C Diffusion coefficient of carbon in austenite D = cm s 1 Coefficient β = o C 1 Equilibrium temperature of the graphite eutectic Cementite eutectic formation temperature ΔT sc = T s T c T s = Si 14.88P T c = (C 3.33Si 1.58P), o C ΔT sc = C Si +36.9P, o C Eutectic density ρ e = 0.96ρ γ ρ gr, g cm 3 Austenite density ρ γ = 7.51 g cm 3 Graphite density ρ gr =. g cm 3 Melt density ρ l = 7.1 g cm 3 Average temperature of the metal just after pouring in the mold cavity T i = 150 o C The influence of the nucleation coefficients on the nodule count is shown in Figure 8. The calculations made for nodule count were based on Eqs. (61) (63). From Figure 8, it is apparent that the nodule count increases when b decreases and N s increases. In addition, it is well known [11] that for given cooling rate prolonged bath holding time leads to reduction in N s and to an increase in b parameter. Consequently, prolonged bath holding time leads to a reduction in the nodule count. According to Eq. (15) the cooling rate increases as the ability of the mold to absorb heat a increases and as the casting modulus M decreases. The cooling rate is also dependent on the B parameter (Eq. 14), and hence on the initial temperature T i of the cast iron just after pouring into the mould. It also depends on the equilibrium eutectic temperature T s and the specific heat c (Eq. (15). Figure 9 shows the effect of B and of the a/m ratios on the cooling rate at the onset of eutectic solidification. A schematic diagram showing the role of various technological factors on the nodule count in ductile cast iron is given in Figure
18 a) b) Fig. 8. Influence of the nucleation coefficient on the nodule count: a) N s = cm 3 ; b) b = 60 o C (rest of data see Fig. 7) Fig. 9. Effect of B (T i, T s ) and a/m ratio on the cooling rate Q 130
19 Nodule count N Cooling rate Q Diffusion coefficient D Nucleation coefficients N s, b Initial temperature of melt T i Casting modulus M Mould material a Chemical composition of bath Furnace slag and atmosphere Spheroidizing and inoculation practice Temperature and holding time of bath Technological factors Fig. 10. Effect of technological factors on the nodule count in ductile cast iron 4. CHILLING TENDENCY Since ΔT m = T s T m, a plot of the function T m = f (Q) using Eqs. (60) and (61) is given in Figure 11. From this figure, it is found that the minimum temperature for the solidification of the graphite eutectic T m levels with the temperature T c when the cooling rate, Q = Q cr and ΔT m = T s T c = ΔT sc, so below T c, the solidification of cementite eutectic begins. By taking into account this condition into Eqs. (60) and (61) and using Eq. (15) an expression is derived for the critical casting modulus M cr = (V/F) cr below which a chill is likely to develop in castings Mcr = pcr CT (65) where the coefficient p cr includes the parameters (a, z, B T s ) related to the cast iron cooling rates 4) p cr 3 T s = a π β z B Le c 1/6 (66) 4) Influence of L e and c can be neglected. 131
20 Fig. 11. Influence of the cooling rate Q on the minimal solidification temperature T m for graphite eutectic (rest of data see Fig. 7) CT is the chilling tendency for ductile cast iron 1 1 b CT = exp 1/ D N T s βδt Δ sc sc 1/3 (67) From Eqs. (57) and (67), for ΔT m = ΔT sc, CT can be simplified to 1/3 1 1 CT = 1/ D N T βδ sc (68) Typical CT values range from 0.8 to 1. s 1/ / o C 1/3. The influence of the various terms on CT, (Eq. (68)) can be summarized as: Diffusion coefficient, as D increases, CT decreases. The temperature range ΔT sc = T s T c, depends on the chemical composition as o Δ = C Si P, C (69) T sc In particular, carbon reduces ΔT sc while silicon expends it (Fig. 1a). The effect of this range on CT is shown in Figure 1b. Notice from this figure that CT decreases with increasing ΔT sc ranges. The Nucleation susceptibilities of graphite depends on the resultant values of N s and b (see previous section). In particular, CT increases with increasing b and decreasing N s (Fig. 13). 13
21 a) b) Fig. 1. Influence of carbon and silicon on: a) ΔT sc ; b) ΔT sc on the chilling tendency CT Fig. 13. Influence of N s and b on the chilling tendency of ductile cast iron; ΔT sc = 60 o C (rest of data see Fig. 7) 5. CHILL In establishing the chill of cast iron, it is common to implement a set of chill tests on castings, which consist of plates with different wall thicknesses, thus the critical casting modulus can be determined from M cr V = F cr cr (70) where V cr and F cr are chilled volume and surface area of casting. 133
22 Clill s cr Influence on cooling rate Temperature range ΔT ec Chilling tendency CT Diffusion coefficient D Nodule count N Nucleation parameters N s, b Initial temperature of melt T i Mould Material a Eutecic temperature T e Chemical composition of bath Furnace slag and atmosphere Spheroidizing and inoculation practice Temperature and holding time of bath Technological factors Fig. 14. Effect of technological factors on the chill and chilling tendency of ductile iron For plates with wall thickness, s and lengths and widths which easily exceed s, M cr = = V cr /F cr = (s cr F cr )/( F cr ), and the critical wall thickness s cr below which the chill forms is scr = Mcr (71) and after using Eq. (65) scr = pcr CT (7) From Eqs. (66), (67) and (7) results a diagram showing the influence of technological factors on chilling tendency CT and the chill of ductile cast iron is shown in Figure CONCLUSIONS A theoretical analysis is proposed for the solidification of ductile cast iron which allows to predict nodule counts based only on the knowledge of cooling rates and chemical composition, the initial temperature of the metal just after pouring into the mould, the diffu 134
23 sion coefficient of carbon in austenite and the graphite nucleation coefficients. From the proposed theory, expressions are derived for the chilling tendency and chill of cast iron. A summary of the present analysis on the nodule count of cast iron indicates that it depends on: The chemical composition of the cast, through D, N s, and b. The inoculation practice, the bath superheating temperature and time, furnace slag and atmosphere, through N s and b. Cooling rate, through M, a and B. The chilling tendency CT of the nodular cast iron depends on: Chemical composition through D, ΔT sc, N s, and b, Inoculation and spheroidization practice, superheat temperature and time, as well as furnace slag and atmosphere through N s and b. In addition, the chill of the nodular cast iron is related to cooling rate Q and CT. REFERENCES [1] Jincheng Liu, Elliot R.: The influence of cast structure on the austempering of ductile iron. International Journal of cast Metals Researches, 11 (1999), p. 407 [] Lesoult G., Castro M., Lacaze J.: Solidification of Spheroidal Graphite Cast Iron: III Microsegregation related effects. Acta Materialia, 47 (1999), p [3] Achmadabadi M.N., Niyama E., Ohide T.: Structural control of 1% Mn aided by modeling of microsegregation. Transactions of the American Foundrymans Society, 97 (1994), p. 69 [4] Javaid A., Thompson J., Davis K.G.: Critical conditions for obtaining carbide free microstrucutre in thinwall ductile iron. AFS Transactions, 10 (00), p. 889 [5] Javaid A., Thompson J., Sahoo M., Davis K.G.: Factors affecting formation of carbides in thinwll DI castings, AFS Transactions, 99 (1999), p. 441 [6] Fraœ E., Lopez H.: Generation of International Pressure During Solidification of Eutectic Cast Iron. Transactions of the American Foundryman Society, 10 (1994), p. 597 [7] Fraœ E., Podrzucki C.: Inoculated Cast Iron. AGH, Cracov, 1981 [8] Venugopalan D.: A Kinetic Model of the γ α + Gr Eutectoid Transformation in Spheroidal Graphite Cast Iron. Metallurgical and Materials Transactions, 1 A (1990), p. 913 [9] Chvorinov N.: Theorie der Erstarrung von Gusstûcken. Die Giesserei (1940) 7, p. 10 [10] Fras E., Lopez H.: A theoretical analysis of the chilling suspectibility of hypoeutectic FeC alloys. Acta Metallurgica and Materialia, 41 (1993) 1, p [11] Fras E., Górny M., Lopez H., Tartera J.: Nucleation and grains density in grey cast iron. A theoretical model and experimental verification. International Journal of Cast Metals Research, 16 (003), pp [1] Wojnar L.: Effect of graphite size and distribution on fracture and fractography of ferritic nodular cast iron. Acta Stereologica, 5/ (1986), p
24 [13] Wiencek K., Ryœ J.: The estimation of Fe 3 C particle density in steel by simple counting measurements made in plan sections. Materialas Engineering (1998) 3, p. 396 [14] Merchant H.D.: Solidification of Cast Iron, Recent Research on Cast iron. Gordon and Breach, Science Publishers, NewYork, 1968 [15] Agren J.: A revised expression for the diffusivity of carbon in binary FeC austenite. Scripta Metallurgica, 0 (1986), p Received March
DOE FUNDAMENTALS HANDBOOK
DOEHDBK1019/293 JANUARY 1993 DOE FUNDAMENTALS HANDBOOK NUCLEAR PHYSICS AND REACTOR THEORY Volume 2 of 2 U.S. Department of Energy Washington, D.C. 20585 FSC6910 Distribution Statement A. Approved for
More informationPitting Corrosion of Metals A Review of the Critical Factors
Journal of the Electrochemical Society, Vol. 145, No. 6, 1998, pp. 21862198. ISSN: (Print 00134651) (Online 19457111) DOI: 10.1149/1.1838615 http://www.electrochem.org/ http://scitation.aip.org/jes
More informationPROPAGATION OF SOUND WAVES IN DUCTS
PROPAGATION OF SOUND WAVES IN DUCTS Finn Jacobsen Acoustic Technology, Department of Electrical Engineering Technical University of Denmark, Building 352 Ørsteds Plads, DK2800 Lyngby Denmark fja@elektro.dtu.dk
More informationEPSRC Research Project EP/G00028X/1. Environmental Assessment of Domestic Laundering. Final Modelling Report
ESRU Report EPSRC Research Project EP/G00028X/1 Environmental Assessment of Domestic Laundering Final Modelling Report Kelly N J K, Markopoulos A and Strachan P A March 2012 Energy Systems Research Unit
More informationAlN Thin Film Electroacoustic Devices
Comprehensive Summaries of Uppsala Dissertations from the Faculty of Science and Technology 817 AlN Thin Film Electroacoustic Devices BY GONZALO FUENTES IRIARTE ACTA UNIVERSITATIS UPSALIENSIS UPPSALA 2003
More informationAIR SYSTEM BASICS. form the groundwork for the design, installation, operation, troubleshooting of these systems. Air duct Manometer
... AIR SYSTEM BASICS One of the fundamental concepts that apply to air systems is the fluid mechanics of conveying air. This article presents the basic principles that form the groundwork for the design,
More informationAxial Flow Compressor Mean Line Design
Axial Flow Compressor Mean Line Design Niclas Falck February 2008 Master Thesis Division of Thermal Power Engineering Department of Energy Sciences Lund University, Sweden Niclas Falck 2008 ISSN 02821990
More informationMathematical modeling of human brain physiological data
Mathematical modeling of human brain physiological data Dissertation zur Erlangung des Doktorgrades der Naturwissenschaften (Dr. rer. nat.) der Naturwissenschaftlichen Fakultät für Physik der Universität
More informationHigh Strain R. 33. High Strain Rate and Impact Experiments. Part D 33
1 High Strain R 33. High Strain Rate and Impact Experiments Part D 33 K. T. Ramesh Experimental techniques for highstrainrate measurements and for the study of impactrelated problems are described. An
More informationDynamic Effect in the Capillary Pressure Saturation Relationship and its Impacts on Unsaturated Flow
Dynamic Effect in the Capillary Pressure Saturation Relationship and its Impacts on Unsaturated Flow S. Majid Hassanizadeh,* Michael A. Celia, and Helge K. Dahle ABSTRACT Capillary pressure plays a central
More informationAcidbase Chemistry of Aquatic Systems
i Acidbase Chemistry of Aquatic Systems An introduction to the chemistry of acidbase equilibria with emphasis on the carbon dioxide system in natural waters eith A. Hunter Professor in Chemistry Department
More informationSensing and Control. A Process Control Primer
Sensing and Control A Process Control Primer Copyright, Notices, and Trademarks Printed in U.S.A. Copyright 2000 by Honeywell Revision 1 July 2000 While this information is presented in good faith and
More informationExperimental investigation and CFD simulation of organic peroxide pool fires (TBPB and TBPEH)
Experimental investigation and CFD simulation of organic peroxide pool fires (TBPB and TBPEH) Von der Fakultät für Ingenieurwissenschaften, Abteilung Maschinenbau und Verfahrenstechnik der Universität
More informationColloidal Suspensions in Temperature Gradients with Mesoscopic Simulations
Colloidal Suspensions in Temperature Gradients with Mesoscopic Simulations I n a u g u r a l  D i s s e r t a t i o n zur Erlangung des Doktorgrades der MathematischNaturwissenschaftlichen Fakultät der
More informationGuidelines to Determine SiteSpecific Parameters for Modeling the Fate and Transport of Monoaromatic Hydrocarbons in Groundwater
Guidelines to Determine SiteSpecific Parameters for Modeling the Fate and Transport of Monoaromatic Hydrocarbons in Groundwater Submitted to: Scott Scheidel, Administrator IOWA COMPREHENSIVE PETROLEUM
More informationPYROLYSISGAS CHROMATOGRAPHY
ALMA MATER STUDIORUMUNIVERSITY OF BOLOGNA DEPARTMENT OF CHEMISTRY G. CIAMICIAN Ph. D. COURSE IN CHEMICAL SCIENCE COURSE XXIV Afference sector: CHIM/03A1 Scientificdisciplinary sector: CHIM/01 PYROLYSISGAS
More informationField Estimation of Soil Water Content
Field Estimation of Soil Water Content A Practical Guide to Methods, Instrumentation and Sensor Technology VIENNA, 2008 TRAINING COURSE SERIES30 TRAINING COURSE SERIES No. 30 Field Estimation of Soil Water
More informationApplication of CFD in Membrane Technique
Application of CFD in Membrane Technique Der Fakultät für Ingenieurwissenschaften, Abteilung Maschinenbau der Universität DuisburgEssen zur Erlangung des akademischen Grades DOKTORINGENIEUR genehmigte
More informationFORSCHUNGSZENTRUM ROSSENDORF Institut fur Ionenstrahlphysik und Materialforschung Modeling and Computer Simulation of Ion Beam Synthesis of Nanostructures von der Fakultat Mathematik und Naturwissenschaften
More information* Corresponding author: turng@engr.wisc.edu
Quantitative Study of the Dimensional Stability of Injection Molded Parts Using Conventional and Microcellular Injection Molding and Microcellular CoInjection Molding Adam Kramschuster, Ryan Cavitt, Chris
More informationInstitut für Ernährungs und Lebensmittelwissenschaften. Investigations into the HighTemperature Air Drying of Tomato Pieces
Institut für Ernährungs und Lebensmittelwissenschaften Investigations into the HighTemperature Air Drying of Tomato Pieces InauguralDissertation zur Erlangung des Grades DoktorIngenieur (Dr.Ing.)
More informationThe Scattering of α and β Particles by Matter and the Structure of the Atom
E. Rutherford, Philos. Mag, 6, 21 1911 The Scattering of α and β Particles by Matter and the Structure of the Atom E. Rutherford University of Manchester 1 (Received April 1911) 1 It is well known that
More informationSYNTHESIS AND PROPERTIES OF NEW SEMICONDUCTOR ALLOYS FOR LONG WAVELENGTH COHERENT EMITTERS ON GALLIUM ARSENIDE
UNIVERSITÀ DEGLI STUDI DI TRIESTE XVI CICLO DEL DOTTORATO DI RICERCA IN FISICA SYNTHESIS AND PROPERTIES OF NEW SEMICONDUCTOR ALLOYS FOR LONG WAVELENGTH COHERENT EMITTERS ON GALLIUM ARSENIDE DOTTORANDO
More informationSpecific volume of polymers. Influence of the thermomechanical history
Specific volume of polymers Influence of the thermomechanical history CIPDATA LIBRARY TECHNISCHE UNIVERSITEIT EINDHOVEN Beek, Maurice H.E. van der Specific volume of polymers : influence of the thermomechanical
More informationREMARKS ON SURFACE INTEGRITY OF ELECTRIC DISCHARGE MACHINED SURFACES: A STATE OF ART REVIEW
REMARKS ON SURFACE INTEGRITY OF ELECTRIC DISCHARGE MACHINED SURFACES: A STATE OF ART REVIEW Bülent EKMEKÇİ, bekmekci@hotmail.com Karaelmas University, 67100, Zonguldak, Turkey Abdulkadir ERDEN, aerden@atilim.edu.tr
More informationAn implicit level set method for modeling hydraulically driven fractures
Available online at www.sciencedirect.com Comput. Methods Appl. Mech. Engrg. 197 (28) 2858 2885 www.elsevier.com/locate/cma An implicit level set method for modeling hydraulically driven fractures Anthony
More informationHALL EFFECT SENSING AND APPLICATION
HALL EFFECT SENSING AND APPLICATION MICRO SWITCH Sensing and Control 7DEOHRI&RQWHQWV Chapter 1 Hall Effect Sensing Introduction... 1 Hall Effect Sensors... 1 Why use the Hall Effect... 2 Using this Manual...
More informationUG219 TRAMAQ  cold start emissions. Summary report
UG219 TRAMAQ  cold start emissions. Summary report DCW Blaikley AP Smith EA Feest AH Reading May 2001 UG219 TRAMAQ cold start emissions. Summary report DCW Blaikley AP Smith EA Feest AH Reading May 2001
More informationInterfacial conditions between a pure fluid and a porous medium: implications for binary alloy solidification
J. Fluid Mech. (26), vol. 55, pp. 149 173. c 26 Cambridge University Press doi:1.117/s2211257998 Printed in the United Kingdom 149 Interfacial conditions between a pure fluid and a porous medium: implications
More informationFR I CTI 0 N SURFACE PHENOMENA
FR I CTI 0 N SURFACE PHENOMENA TRIBOLOGY SERIES Editor D. Dowson (Gt. Britain) Advisory Board W.J. Bartz (Germany) R. Bassani (Italy) B. Briscoe (Gt. Britain) H. Czichos (Germany) K. Friedrich (Germany)
More information